Solvothermal synthesis of uniform bismuth nanospheres using poly(N-vinyl-2-pyrrolidone) as a reducing agent
© Wu et al; licensee Springer. 2011
Received: 26 July 2010
Accepted: 12 January 2011
Published: 12 January 2011
Uniform bismuth nanospheres were successfully prepared from bismuth nitrate in the presence of poly(N-vinyl-2-pyrrolidone) (PVP) by solvothermal process. The product was characterized by powder X-ray diffraction, scanning electron microscopy, transmission electron microscopy, selected area electron diffraction, and energy-dispersive X-ray. PVP plays a critical role both as a reducing agent and a capping agent in the formation of bismuth nanospheres. Shape and size of bismuth nanospheres could be tuned by changing the employed PVP/bismuth salt ratio. It was also found the solvent had an effect on the morphologies of bismuth nanomaterials. The possible formation and growth mechanism of bismuth nanospheres were also discussed and proposed to explain the reduction step.
Recently, metal nanostructures with functional properties have been extensively studied due to their wide applications. Among the various metal nanostructures, monodisperse metallic nanospheres have attracted considerable attention because of their unique optical, catalytic, as well as novel chemical and biological properties [1–8]. For example, the controlled silver nanospheres were applied for optical studies and antibacterial applications [9, 10]. Thus, much effort has been devoted to the preparation of new metal nanospheres and their functional transformation [11–14]. As a semimetal, bismuth has unusual properties due to its highly anisotropic Fermi surface, low carrier densities, small carrier effective masses, and long carrier mean free path . Bismuth nanostructures have received steadily growing interests, since they play important roles in many diverse applications [16, 17]. Different bismuth nanomaterials, such as single-crystal bismuth thin film and nanowire, have been investigated for their large magnetoresistance, finite-size effects, and enhanced thermal conductivity [18–20]. It was also reported that spherical bismuth nanomaterials were a good catalyst for the growth of SnS2 nanotubes and germanium nanowires [21, 22]. Up to now, a wide variety of bismuth nanostructures such as nanoparticles , nanowires , nanorods , nanotubes [26–28], triangular nanoplates , bunch-like nanostructures , nanocubes , as well as nanospheres (>100 nm) [31–34] have been prepared by using different methods. Among these methods, solvothermal synthesis has become an important and promising approach to prepare controlled inorganic nanocrystals [35–37].
In the reported literatures, the alcohol [normally ethylene glycol (EG)] was used as both solvent and reducing agent to generate bismuth nanospheres with a wide size distribution [31–34]. Wang and Xia  have developed the synthesis of uniform bismuth nanospheres by thermal decomposition bismuth acetate in EG under the protection of nitrogen. The use of protection of inactive gas and organic metal precursor, however, made it complicated and costly. Hence, a simple, low-cost approach for the preparation of uniform bismuth nanospheres is highly desired.
In this communication, we describe a solvothermal process for the synthesis of uniform bismuth nanospheres in the presence of poly(N-vinyl-2-pyrrolidone) (PVP). In most cases, PVP was used as a protecting agent to cap and stabilize the particles to avoid aggregation in the solution . It was also reported that PVP was used as reducing agent in the preparation of noble metallic nanostructures [40, 41]. In this synthesis, PVP acts as both reducing and capping agent. To the best of our knowledge, there are few publications relevant to the synthesis of bismuth nanomaterials using PVP as a reducing agent.
Bismuth nitrate pentahydrate (Bi(NO3)3·5H2O) was purchased from Fuchen Chemicals Reagent (China). N,N-dimethylformamide (DMF), ammonia, mannitol, and EG were purchased from Sinopharm Chemical Reagent (China); PVP (with average M w of 10,000) was purchased from Sigma-Aldrich Inc. All the reagents were analytical grade and used directly without further purification.
Synthesis of uniform bismuth nanospheres
Experimental conditions for the synthesis of bimuth nanomaterials
The amount of PVP (g)
The bismuth nanostructures were characterized by powder X-ray diffraction (XRD), scanning electron microscopy (SEM), transmission electron microscopy (TEM), selected area electron diffraction (SAED), and energy-dispersive X-ray (EDX). The powder XRD pattern was recorded on Bruker AXS D8 Discover (Cu Kα radiation, λ = 1.5406 Å). The scanning rate is 1°/min in the 2θ range from 20 to 70°. The SEM images were taken on a Hitachi S4800 field emission scanning electron microscope operating at 3 or 5 kV (FESEM, Japan). TEM images and SAED pictures were recorded on a Philips Technai G2 20 electron microscope (Manufacturer: FEI Company), using an accelerating voltage of 200 kV. The EDX analysis was performed on an Oxford Instruments Inca with a scanning range from 0 to 20 keV. The samples for TEM observations were prepared by dispersing some of the solid products into absolute alcohol and then sonicated for several minutes. A few drops of the suspension were deposited on the copper grid, which was then put into the desiccator. The thermogravimetric and differential analysis was done by DIAMOND TG/DTA instrument (PerkinElmer Instruments, Waltham, CT, USA) with a heating rate of 10°C/min.
Results and discussion
The morphologies and structures of the as-prepared bismuth nanospheres were investigated by SEM and TEM images. Figure 1b, c, d shows the representative SEM images of the as-prepared bismuth nanospheres with different magnifications. The low-magnification images (Figure 1b, c) indicate the large production of uniform bismuth nanospheres. No other bismuth morphologies could be found in the whole sample. The diameters of these nanospheres varied from 160 to 210 nm and most of them were about 180 nm. The high-magnification image shown in Figure 1d clearly reveals the detailed morphologies of the products, indicating the formation of uniform, regular nanospheres with smooth surfaces.
In this study, it was found that there was no black product precipitated from the solution in the absence of PVP under identical experiment condition. The XRD pattern of the obtained white product could not be assigned in the XRD standard data base (Figure S3 in Additional File 3). It is obvious that PVP plays a key role in the formation of bismuth nanospheres. It was proposed that PVP reduced Bi3+ ions to give metallic bismuth. The reduction process could be probably understood considering two main reactions: (1) direct abstraction of hydrogen atoms from the polymer by the Bi3+ ions; (2) reduction of the Bi3+ ions by the organic radicals formed in (1) or during the bismuth-accelerated degradation of PVP, which is similar to the reported literatures [40, 42]. It was reported that the capping organic molecules in the reaction system could determine the subsequent morphology of the product because of their special chemical properties and self-assembling functions [43–45]. Recently, it was also found that EG molecules could adsorb onto the surface of bismuth crystals through O-Bi bonding which could significantly decrease their growth rates and lead to highly anisotropic growth [33, 46]. Thus, when the molar ratio of repeating units of PVP to Bi3+ is about 3, that is, there is no excess PVP in the solution, these uniform bismuth nanospheres can be obtained under the only effect of EG.
Interestingly, when DMF was instead of EG, bismuth nanoparticles and nanotubes arrays were formed under identical experimental conditions (Figure 4c, d). The average diameter of bismuth nanoparticles is about 50 nm, and the diameters of the bismuth nanotubes are in a narrow range from about 3.2 to 5.2 nm, with an average diameter of 4.3 nm. EDX was used to further analyze the elemental compositions of these nanotubes lying on the hole of the copper grid. It reveals the elemental Bi signals and confirmed the purity of this bismuth nanotube (Figure 4f). The copper and carbon peaks are due to the carbon-coated copper grid. Here, DMF plays an important role in the fabrication of bismuth nanotubes. In this synthesis, the starting materials can dissolve in DMF and DMF can partially decompose into dimethylamine, which is a good coordination ligand with N-chelation. The diffusion of Bi3+ ions in DMF-dimethylamine will be faster due to its lower viscosity, which is beneficial for the formation of nanotube products . The formation mechanism is still limited and further study in progress.
In summary, uniform bismuth nanospheres were successfully synthesized via a facile solvothermal process by reduction of EG solution of bismuth salt, using PVP both as a reducing agent and a capping agent. The shapes and sizes of the bismuth nanostructures varied with the changing of the PVP/bismuth salt molar ratio. Uniform bismuth nanospheres with an average diameter of 180 nm could be routinely synthesized through this solvothermal approach by controlling the PVP/bismuth salt ratio. The solvent EG also played an important role in the formation of uniform bismuth nanospheres. Bismuth nanoparticles and nanotubes were formed when DMF was used as a solvent instead of EG. The possible formation mechanism of the bismuth nanotubes was also discussed and further study was in progress.
selected area electron diffraction
scanning electron microscopy
transmission electron microscopy
This study was supported by National Natural Science Foundation of China (Grant 20801043), the Program for New Century Excellent Talents in University (NCET-09-0136), and the Outstanding Youth Scientific Foundation of Hubei Province (2009CDA075).
- Bigall NC, Härtling T, Klose M, Simon P, Eng LM, Eychmüller A: Monodisperse platinum nanospheres with adjustable diameters from 10 to 100 nm: Synthesis and distinct optical properties. Nano Lett 2008, 8: 4588. 10.1021/nl802901tView ArticleGoogle Scholar
- Schwartzberg AM, Olson TY, Talley CE, Zhang JZ: Synthesis, characterization, and tunable optical properties of hollow gold nanospheres. J Phys Chem B 2006, 110: 19935. 10.1021/jp062136aView ArticleGoogle Scholar
- Semagina N, Kiwi-Minsker L: Palladium nanohexagons and nanospheres in selective alkyne hydrogenation. Catal Lett 2009, 127: 334. 10.1007/s10562-008-9684-1View ArticleGoogle Scholar
- Lee S, Chon H, Lee M, Choo J, Shin SY, Lee YH, Rhyu IJ, Son SW, Oh CH: Surface-enhanced raman scattering imaging of HER2 cancer markers overexpressed in single MCF7 cells using antibody conjugated hollow gold nanospheres. Biosens Bioelectron 2009, 24: 2260. 10.1016/j.bios.2008.10.018View ArticleGoogle Scholar
- Nitin N, Javier DJ, Roblyer DM, Richards-Kortum R: Widefield and high-resolution reflectance imaging of gold and silver nanospheres. J Biomed Opt 2007, 12: 051505. 10.1117/1.2800314View ArticleGoogle Scholar
- Skala MC, Crow MJ, Wax A, Izatt JA: Photothermal optical coherence tomography of epidermal growth factor receptor in live cells using immunotargeted gold nanospheres. Nano Lett 2008, 8: 3461. 10.1021/nl802351pView ArticleGoogle Scholar
- Li W, Camargo PHC, Lu X, Xia Y: Dimers of silver nanospheres: Facile synthesis and their use as hot spots for surface-enhanced raman scattering. Nano Lett 2008, 9: 485. 10.1021/nl803621xView ArticleGoogle Scholar
- Chon H, Lee S, Son SW, Oh CH, Choo J: Highly sensitive immunoassay of lung cancer marker carcinoembryonic antigen using surface-enhanced raman scattering of hollow gold nanospheres. Anal Chem 2009, 81: 3029. 10.1021/ac802722cView ArticleGoogle Scholar
- Cobley CM, Rycenga M, Zhou F, Li ZY, Xia Y: Controlled etching as a route to high quality silver nanospheres for optical studies. J Phys Chem C 2009, 113: 16975. 10.1021/jp906457fView ArticleGoogle Scholar
- Lok C-N, Ho C-M, Chen R, He Q-Y, Yu W-Y, Sun H, Tam PK-H, Chiu J-F, Che C-M: Proteomic analysis of the mode of antibacterial action of silver nanoparticles. J Proteome Res 2006, 5: 916. 10.1021/pr0504079View ArticleGoogle Scholar
- Jia FL, Zhang LZ, Shang XY, Yang Y: Non-aqueous sol-gel approach towards the controllable synthesis of nickel nanospheres, nanowires, and nanoflowers. Adv Mater 2008, 20: 1050. 10.1002/adma.200702159View ArticleGoogle Scholar
- Goy-López S, Castro E, Taboada P, Mosquera Vc: Block copolymer-mediated synthesis of size-tunable gold nanospheres and nanoplates. Langmuir 2008, 24: 13186.View ArticleGoogle Scholar
- Xiao C-W, Shen C-M, Xu Z-C, Yang T-Z, Gao H-J: Anomalous aggregation growth of palladium nanosphere with spr band in visible range. Chin Phys B 2008, 17: 2066. 10.1088/1674-1056/17/6/021View ArticleGoogle Scholar
- Lee C-L, Kuo L-C, Huang Y-C, Yen Y-W: Mesoporous, self-assembled palladium nanospheres: High efficiency activator for electroless nickel deposition. Electrochem Commun 2006, 8: 697. 10.1016/j.elecom.2006.02.023View ArticleGoogle Scholar
- Yang FY, Liu K, Chien CL, Searson PC: Large magnetoresistance and finite-size effects in electrodeposited single-crystal Bi thin films. Phys Rev Lett 1999, 82: 3328. 10.1103/PhysRevLett.82.3328View ArticleGoogle Scholar
- Carotenuto G, Hison C, Capezzuto F, Palomba M, Perlo P, Conte P: Synthesis and thermoelectric characterisation of bismuth nanoparticles. J Nanoparticle Res 2009, 11: 1729. 10.1007/s11051-008-9541-6View ArticleGoogle Scholar
- Zhang Z, Yu K, Bai D, Zhu Z: Synthesis and electrochemical sensing toward heavy metals of bunch-like bismuth nanostructures. Nanoscale Res Lett 2010, 5: 398. 10.1007/s11671-009-9495-3View ArticleGoogle Scholar
- Boukai A, Xu K, Heath JR: Size-dependent transport and thermoelectric properties of individual polycrystalline bismuth nanowires. Adv Mater 2006, 18: 864. 10.1002/adma.200502194View ArticleGoogle Scholar
- Huber TE, Nikolaeva A, Gitsu D, Konopko L, Graf MJ: Role of boundary roughness in the electronic transport of Bi nanowires. J Appl Phys 2008, 104: 123704. 10.1063/1.3041491View ArticleGoogle Scholar
- Moore AL, Pettes MT, Zhou F, Shi L: Thermal conductivity suppression in bismuth nanowires. J Appl Phys 2009, 106: 034310. 10.1063/1.3191657View ArticleGoogle Scholar
- Yella A, Mugnaioli E, Panthöfer M, Therese HA, Kolb U, Tremel W: Bismuth-catalyzed growth of SnS 2 nanotubes and their stability. Angew Chem Int Ed 2009, 48: 6426. 10.1002/anie.200900546View ArticleGoogle Scholar
- Xiang Y, Cao L, Arbiol J, Brongersma ML, Fontcuberta i Morral A: Synthesis parameter space of bismuth catalyzed germanium nanowires. Appl Phys Lett 2009, 94: 163101. 10.1063/1.3116625View ArticleGoogle Scholar
- Wang F, Tang R, Yu H, Gibbons PC, Buhro WE: Size- and shape-controlled synthesis of bismuth nanoparticles. Chem Mater 2008, 20: 3656. 10.1021/cm8004425View ArticleGoogle Scholar
- Xu Y, Ren Z, Ren W, Cao G, Deng K, Zhong Y: Magnetic-field-assisted solvothermal growth of single-crystalline bismuth nanowires. Nanotechnology 2008, 19: 115602. 10.1088/0957-4484/19/11/115602View ArticleGoogle Scholar
- Cao S, Guo C, Wang Y, Miao J, Zhang Z, Liu Q: Template-catalyst-free growth of single crystalline bismuth nanorods by RF magnetron sputtering method. Solid State Commun 2009, 149: 87. 10.1016/j.ssc.2008.10.003View ArticleGoogle Scholar
- Yang D, Meng G, Xu Q, Han F, Kong M, Zhang L: Electronic transport behavior of bismuth nanotubes with a predesigned wall thickness. J Phys Chem C 2008, 112: 8614. 10.1021/jp8008892View ArticleGoogle Scholar
- Derrouiche S, Zoican Loebick C, Wang C, Pfefferle L: Energy-induced morphology changes in bismuth nanotubes. J Phys Chem C 2010, 114: 4336. 10.1021/jp911039jView ArticleGoogle Scholar
- Boldt R, Kaiser M, Köhler D, Krumeich F, Ruck M: High-yield synthesis and structure of double-walled bismuth-nanotubes. Nano Lett 2010, 10: 208. 10.1021/nl903291jView ArticleGoogle Scholar
- Fu R, Xu S, Lu Y-N, Zhu JJ: Synthesis and characterization of triangular bismuth nanoplates. Cryst Growth Des 2005, 5: 1379. 10.1021/cg049686nView ArticleGoogle Scholar
- Wang WZ, Poudel B, Ma Y, Ren ZF: Shape control of single crystalline bismuth nanostructures. J Phys Chem B 2006, 110: 25702. 10.1021/jp063474eView ArticleGoogle Scholar
- Cheng G, Wu J, Xiao F, Yu H, Lu Z, Yu X, Chen R: Synthesis of bismuth micro- and nanospheres by a simple refluxing method. Mater Lett 2009, 63: 2239. 10.1016/j.matlet.2009.07.045View ArticleGoogle Scholar
- Li J, Fan H, Chen J, Liu L: Synthesis and characterization of poly(vinyl pyrrolidone)-capped bismuth nanospheres. Colloids Surf A 2009, 340: 66. 10.1016/j.colsurfa.2009.03.007View ArticleGoogle Scholar
- Wang J, Wang X, Peng Q, Li Y: Synthesis and characterization of bismuth single-crystalline nanowires and nanospheres. Inorg Chem 2004, 43: 7552. 10.1021/ic049129qView ArticleGoogle Scholar
- Wu J, Yang H, Li H, Lu Z, Yu X, Chen R: Microwave synthesis of bismuth nanospheres using bismuth citrate as a precursor. J Alloys Compd 2010, 498: L8. 10.1016/j.jallcom.2010.03.165View ArticleGoogle Scholar
- Wang X, Zhuang J, Peng Q, Li Y: A general strategy for nanocrystal synthesis. Nature 2005, 437: 121. 10.1038/nature03968View ArticleGoogle Scholar
- Nikolopoulou A, Papoulis D, Komarneni S, Tsolis-Katagas P, Panagiotaras D, Kacandes GH, Zhang P, Yin S, Sato T: Solvothermal preparation of TiO 2 /saponite nanocomposites and photocatalytic activity. Appl Clay Sci 2009, 46: 363. 10.1016/j.clay.2009.09.007View ArticleGoogle Scholar
- Gao F, Lu Q, Komarneni S: Interface reaction for the self-assembly of silver nanocrystals under microwave-assisted solvothermal conditions. Chem Mater 2005, 17: 856. 10.1021/cm048663tView ArticleGoogle Scholar
- Wang Y, Xia Y: Bottom-up and top-down approaches to the synthesis of monodispersed spherical colloids of low melting-point metals. Nano Lett 2004, 4: 2047. 10.1021/nl048689jView ArticleGoogle Scholar
- Komarneni S, Li D, Newalkar B, Katsuki H, Bhalla AS: Microwave-polyol process for Pt and Ag nanoparticles. Langmuir 2002, 18: 5959. 10.1021/la025741nView ArticleGoogle Scholar
- Hoppe CE, Lazzari M, Pardinas-Blanco I, Lopez-Quintela MA: One-step synthesis of gold and silver hydrosols using poly(N-vinyl-2-pyrrolidone) as a reducing agent. Langmuir 2006, 22: 7027. 10.1021/la060885dView ArticleGoogle Scholar
- Chen J, Lim B, Lee EP, Xia Y: Shape-controlled synthesis of platinum nanocrystals for catalytic and electrocatalytic applications. Nano Today 2009, 4: 81. 10.1016/j.nantod.2008.09.002View ArticleGoogle Scholar
- Kaczmarek H, Kamińska A, Światek M, Rabek JF: Photo-oxidative degradation of some water-soluble polymers in the presence of accelerating agents. Die Angew Makromol Chem 1998, 261–262: 109. 10.1002/(SICI)1522-9505(19981201)261-262:1<109::AID-APMC109>3.0.CO;2-SView ArticleGoogle Scholar
- Bombicz P, Mutikainen I, Krunks M, Leskelä T, Madarász J, Niinistö L: Synthesis, vibrational spectra and X-ray structures of copper(I) thiourea complexes. Inorg Chim Acta 2004, 357: 513. 10.1016/j.ica.2003.08.019View ArticleGoogle Scholar
- Peng X, Manna L, Yang W, Wickham J, Scher E, Kadavanich A, Alivisatos AP: Shape control of CdSe nanocrystals. Nature 2000, 404: 59. 10.1038/35003535View ArticleGoogle Scholar
- Lee S-M, Cho S-N, Cheon J: Anisotropic shape control of colloidal inorganic nanocrystals. Adv Mater 2003, 15: 441. 10.1002/adma.200390102View ArticleGoogle Scholar
- Wang YW, Hong BH, Kim KS: Size control of semimetal bismuth nanoparticles and the UV-visible and IR absorption spectra. J Phys Chem B 2005, 109: 7067. 10.1021/jp046423vView ArticleGoogle Scholar
- Yin Y, Alivisatos AP: Colloidal nanocrystal synthesis and the organic-inorganic interface. Nature 2005, 437: 664. 10.1038/nature04165View ArticleGoogle Scholar
- Alivisatos AP: Semiconductor clusters, nanocrystals, and quantum dots. Science 1996, 271: 933. 10.1126/science.271.5251.933View ArticleGoogle Scholar
- Wei G, Deng Y, Lin Y-H, Nan C-W: Solvothermal synthesis of porous tellurium nanotubes. Chem Phys Lett 2003, 372: 590. 10.1016/S0009-2614(03)00463-9View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.